Download - Hochschule München
2.4.3 Textures Each grain normally has a crystallographic orientation different from that of it neighbor grain. Within an ideal sample, the orientation of all the grains may be randomly distributed in relation to a reference grain. Nevertheless, in the most real specimen the grain order in a preferred orientation, e.g. by the growing process, mechanical treatment or by aligning in groups inside a powder, known as texture. From the XRD diffractogram, the presence of textures can be assumed by comparing the height of the diffraction peaks with those from a database (e.g. ICDD WINPDF), see section 2.4.4. Big differences tend to be a sign of textures. The standard XRD diffraction patterns are measured with a θ/2θ setup, where the lattice planes are orientated parallel to the film surface. In order to determine orientation distribution (texture), all grains within the sample must be measured. This is done by rotating the sample around the azimuth angle 0 360 0 90 - 18 - and the tilt angle for a fixed incident angle θ and reflection angle 2θ. The results from texture measurements are displayed within a pole figure . In this work only a comparison to the PDF file results were done in order to obtain an indication for texture of the carbide grains. 2.4.4 ICDD database WINPDF (Windows Powder Diffraction File) is an International Centre for Diffraction Data (ICDD) database file used for peak identification for individual crystal phases . As constructive interference depends on the distance between the lattice planes, i.e. the crystal structures, and reflection power of the atoms, i.e. the arrangement of the atoms in the unit cell, the reflected diffraction peaks are unique for each material. Within the WINPDF file, data about the reflected diffraction peaks along with corresponding miller indices of any material combination measured, as well as theoretical diffraction peaks of texture free, i.e. ideal powder, have been stored. In addition to the diffraction angles, the relative diffracted intensity for each peak is given. Any irregular intensity distribution in the pattern might be a sign for texture. The used PDF’s in this thesis are: 4-806, 25-1047 for WC, 35-776 for W2C, 20-1316 for WC1-x and 20-1324 for WO3.
2.4.5 Phase characterization Figure 2.7: XRD diffractogram from a 2200K 22% a-C:W film investigated using a θ/2θ scan. Figure 2.7 illustrates a XRD diffractogram, where the scattered intensity is plotted as function of 2θ (scattering angle). On the right axis, the relative intensity of the peaks is shown in relative percentage from. By comparing peak positions with those from the PDF-file, phases can be allocated. Within figure 2.7, peaks can be found around the red lines (WC) and the black (C), whereas no diffraction is observed around peaks from W2C (blue) and WC1-x (green). This means only WC is present within the sample, as the carbon reflection comes from the graphite substrate. In the upper right corner the FWHM of WC peaks around 31° and 35° are show used for calculating the relative crystal size with the Scherrer equation within the sample. Before the FWHM can be calculated, the diffractogram had to be modified using a program (e.g. Analyze), allowing background subtraction, Rachinger correction and smoothing. The Rachinger correction suppresses the Kα2 x-rays from the spectrum. - 19 -